Choose the measure unit in which display the data:
Martensitic Stainless Steel
Description of material
VAL4UK is a martensitic stainless steel with a higher chromium and nickel content than VAL4. Its exhibits high tensile properties combined with a suitable ductility and better corrosion resistance than the common martensitic type 400 series steels thanks to its higher Chromium and Nickel contents. In general, its resistance corrosion is lower to that of type 300 series steels even if in certain environments it could offer the same performance.
Every use where high mechanical properties together with fair values of impact ( toughness) and corrosion resistance are necessary such as dive blades, compressors, pumps, turbines, valves in the oil and gas industries, pump shafts, axles, suspensions, bolting, separation technologies, fasteners, propeller shafts, spindles, homogenizers and centrifuges. It offers good corrosion resistance in mild marine and industrial atmospheres.
Argon Oxygen Decarburization
Any amounts of untemperd martensite must be avoided. Best resistance to either intergranular and stress corrosion is obtained when this grade is in the hardened + tempered or double tempered condition. It’s important to point out that the surface of every kind of stainless steel should be free of contaminants, heat tint, scale and passivated for optimum resistance corrosion. VAL4UK is widely used for dive blades.
Due to high resistance and hardness even in the tempered condition, this grade is not suitable for cold forming such as cold heading. A certain mediocre cold formability could be obtained after a very long lasting annealing and very slow cooling in the furnace.
It is not as good as typical martensitic 400 grades due to its tendency to generate build up edge and long chips because it is not normally supplied in microresulphured condition. Depending on final specific use, a stress relieving after heavy machining process could be useful to avoid deformation of parts. However, it’s important to know that the productivity gain depends on the type of machines used, the kind of tools used and their geometry, cutting fluids and the kind of machine operations on the pieces produced.
This process for martensitic stainless grades is always risky and a special care must be applied in the choice of welding parameters. In any case, if a welding process were required, a preheating is mandatory and the part must be maintained at temperature and followed by immediate annealing or tempering. Fillers of same or close compositions can be used to obtain mechanical properties close to that of the base metal. Alternatively, austenitic fillers may be used considering an inevitable reduction of these properties. In solid state joining such as Friction Welding, VAL4UK provides a quality bond line. When friction welded with different grades, a tempering or annealing of the welded piece must be done in order to soften the martensitic structure of HAZ and bond line.
Blooms and ingots require a suitable preheating to avoid cracks and a slow cooling in the furnace after forging. Overheating must always be avoided in order to reduce the risk of internal bursts and to form a certain amount of ferrite. An improper cooling could result in stress cooling cracks. Large forgings and large cross – section shapes should be left to cool until their core reaches room temperature and, then, immediately, heat treated. A right and suitable heat treatment of pieces after the forging process creates a structure with no or little retained austenite avoiding delayed cracking.
VAL4UK should be double tempered after hardening. Double tempering is not normally used in dive knives where a single one could be sufficient. In any case, depending on required mechanical properties and specific utilizations of final products, quenching and tempering temperatures must be well evaluated in order to optimize impact strength values rather than higher tensile. Obviously, avoiding those temperature ranges able to reduce impact properties and corrosion resistance.